Reaction of Rat Connective Tissue to Implanted Dentin
Braz Dent J (2002) 13(1): 23-26
Tissue reaction to white MTA
Reaction of Rat Connective Tissue to
Implanted Dentin Tubes Filled with a
White Mineral Trioxide Aggregate
Valdir de SOUZA1
Mauro Juvenal NERY1
Italo Medeiros FARACO JÚNIOR2
Pedro Felício Estrada BERNABÉ1
José Arlindo OTOBONI FILHO1
Eloi DEZAN JUNIOR1
of Restorative Dentistry, Faculty of Dentistry of Araçatuba, UNESP, Araçatuba, SP, Brazil
of Pediatric Dentistry, Faculty of Dentistry, Lutheran University of Brazil, Porto Alegre, RS, Brazil
The purpose of this paper was to study the reaction of rat subcutaneous connective tissue to the implantation of dentin tubes filled with
white mineral trioxide aggregate (MTA), a material that will be marketed. The tubes were implanted into rat subcutaneous tissue and
the animals were sacrificed after 7 and 30 days. The undecalcified pieces were prepared for histological analysis with polarized light
and von Kossa technique for mineralized tissues. Granulations birefringent to polarized light and an irregular structure like a bridge
were observed next to the material; both were von Kossa positive. Also, in the dentin wall tubules a layer of birefringent granulations
was observed. The results were similar to those reported for gray MTA, indicating that the mechanisms of action of the white and gray
MTA are similar.
Key Words: mineral trioxide aggregate, subcutaneous tissue implantation.
A mineral trioxide aggregate (MTA) was developed at Loma Linda University for the sealing between
the tooth and the external surfaces (1). Various in vivo
and in vitro investigations have shown good biological
properties of this material (2,3). Deposition of neoformed
hard tissue in direct contact with MTA was observed in
cases of pulp capping (4), pulpotomy (5), repair of
furcal perforations (6), root canal fillings (7) and rootend filling (8).
According Holland et al. (9), the mechanism of
action of MTA, encouraging hard tissue deposition, is
similar to that of calcium hydroxide. Implanting both
materials in subcutaneous connective tissue, they observed granules birefringent to polarized light and next
to these granulations irregular tissue, like a bridge, that
is von Kossa-positive. Torabinejad et al. (10) reported
that MTA has calcium oxide and calcium phosphate in
its composition. In contact with water, calcium oxide
could form calcium hydroxide (9). The calcium ions
from calcium hydroxide react with carbon dioxide from
tissue to form calcite crystals that are birefringent to
polarized light (11,12). Next to these granulations there
is deposition of a hard tissue that is von Kossa-positive
and resembles a bridge (9).
There is a commercially available MTA called
ProRoot MTA (Dentsply, Tulsa, OK, USA) that has a
gray powder. However, Glickman and Koch (13) reported that the manufacturer will place a white ProRoot
MTA on the market. The biological difference between
the gray and the white MTA, when implanted in subcu-
Correspondence: Dr. Roberto Holland, Departamento de Odontologia Restauradora, Faculdade de Odontologia de Araçatuba, UNESP, R. José
Bonifácio 1193, 16015-050, Araçatuba, SP, Brasil. Fax: +55-18-624-8490. e-mail: [email protected]
Braz Dent J 13(1) 2002
R. Holland et al.
taneous tissues is unknown. Thus, the purpose of this
study was to analyze the reaction of rat subcutaneous
connective tissue to the implantation of dentin tubes
filled with white MTA.
von Kossa technique, like a bridge (Figure 2). A highly
birefringent structure was also observed in the interior
of the dentin walls tubules (Figure 3). This structure
formed a layer that was observed at different depths.
MATERIAL AND METHODS
The white MTA (Loma Linda University, Loma
Linda, CA) was prepared in distilled water and introduced
into the root canal of human dentin tubes before being
implanted in the subcutaneous connective tissue. The
dentin tube preparation and the implantation technique
were previously described by Holland et al. (9). The tubes
were implanted in 10 rats and the animals were sacrificed
after 7 and 30 days. The pieces were removed and fixed in
10% buffered formalin solution at pH 7.0. The
undecalcified samples were embedded in paraffin-carnauba wax and serial sections were made at 10 µm
intervals using a hard-tissue microtome, according to
Holland et al. (14). Some sections were stained by the von
Kossa technique for mineralized tissues and other sections, without staining, were examined with a polarized
light microscope to locate the birefringent material.
It may appear that in this paper we studied white
MTA in subcutaneous tissue without a comparative
analysis with a control gray MTA group. In reality the
data presented here are an experimental group of another paper developed in rat subcutaneous connective
tissue (15). That investigation studied the two kinds of
MTA before the material was available commercially.
When we observed that only the gray MTA was on the
market, without any explanation about the matter, we
believed white MTA disappeared for unknown reasons.
The results observed at 7 and 30 days were the
same. For this reason they will be described together.
Numerous large granulations birefringent to polarized
light and von Kossa positive were observed near the
tube opening and generally in contact with the filling
material (Figure 1). Next to these granulations, there
were extensive areas of irregular tissue positive to the
Figure 1. White MTA, 30 days. Note white MTA (F), dentin (D)
and birefringent granulations (G) in direct contact with MTA
(polarized light, 100X).
Braz Dent J 13(1) 2002
Figure 2. White MTA, 30 days. Note dentine (D) and an irregular
tissue like a bridge (arrows) highly positive to the von Kossa
Figure 3. White MTA, 7 days. Observe MTA (F), dentin wall (D)
and a layer (L) of a highly birefringent structure localized in the
dentin tubules (polarized light, 80X).
Tissue reaction to white MTA
In view of this, we decided not to publish the results
with white MTA. However, the paper of Glickman and
Koch (13) gives new life to the white MTA, at least for
us. Thus, the control group of this study is in the
previously published paper (15).
The same results reported by Holland et al.
(9,15) for gray MTA were observed in this experimentation. This fact suggests that some differences in the
materials did not influence the results when they are
implanted in rat subcutaneous connective tissue. The
MTA employed by Holland et al. (9,15) and the one
studied in this experimentation were provided by Dr.
Torabinejad (Loma Linda University). We clinically
observed two differences with these materials: the color
and the setting time, which was greater in the white one.
A large number of papers about MTA were
published in the literature before the material was put
on the market (1-10); however, the color of the material
was not described. Only Faraco (16) compared the two
materials in dog dental pulp. He reported slightly better
results with gray MTA than with white MTA. The
white MTA we studied in this paper was 3 years old and
we do not know how much time the material can be kept
before its properties change.
The deposition of calcite crystals seems to be very
important to the mechanism of action of calcium hydroxide formed after mixing MTA with water. Seux et al. (17)
reported a rich extracellular network of fibronectin in
close contact with these crystals on incubation in a culture
medium without cells. They reported that fibronectin first
came from the culture medium and later from the cells.
The authors concluded that their findings strongly supported the role of calcite crystals and fibronectin as an
initiating step in the formation of a hard tissue barrier. In
our paper we observed a von Kossa-positive tissue barrier
next to these crystals, remembering the hard tissue deposition in direct contact with MTA as described in a series
of papers (6,8). This hard tissue is very irregular in
subcutaneous tissue (9,15) but is similar to dentin in pulp
tissue (4,5) and looks like cementum in furcal perforations (6) and periapical tissues (7).
In conclusion, the observed results and the mechanism of action of white MTA is very similar to those
reported for gray MTA (9,15).
Holland R, Souza V, Nery MJ, Faraco Júnior IM, Bernabé PFE,
Otoboni Filho JA, Dezan Junior E. Reação do tecido conjuntivo
do rato ao implante de tubos de dentina obturados com um
agregado de trióxido mineral branco. Braz Dent J 2002;13(1):2326.
Foi objetivo deste trabalho estudar a reação do tecido conjuntivo
subcutâneo do rato ao implante de tubos de dentina obturados
com MTA branco, material a ser introduzido no mercado. Os
tubos foram implantados no tecido conjuntivo subcutâneo e os
animais sacrificados com 7 e 30 dias de períodos pós-operatório.
As peças não descalcificadas foram preparadas para análise
histológica com luz polarizada e ténica de von Kossa para tecidos
mineralizados. Foi observado junto ao material estudado
granulações birrefringentes à luz polarizada seguida de uma
estrutura irregular, na forma de ponte, ambos von Kossa positivos.
Foi observado também no interior dos túbulos dentinários uma
camada de granulações birrefringentes à luz polarizada. Os
resultados observados são similares aos descritos para o MTA
cinza. Conclui-se que os mecanismos de ação do MTA branco e
cinza são similares.
Unitermos: agregado de trióxido mineral, implante em tecido
1. Lee SJ, Monsef M, Torabinejad M. Sealing ability of a mineral
trioxide aggregate for repair of lateral root perforations. J Endodon
2. Torabinejad M, Hong CU, Pitt Ford TR, Kettering JD. Cytotoxicity of four root end filling materials. J Endodon 1995;21:489492.
3. Torabinejad M, Hong CU, Pitt Ford TR, Kariyawasan SP. Tissue
reaction to implanted Super-EBA and mineral trioxide aggregate
in the mandible of guinea pigs: a preliminary report. J Endodon
4. Pitt Ford TR, Torabinejad M, Abedi HR, Bakland LK,
Kariyawasam SP. Using mineral trioxide aggregate as a pulpcapping material. J Am Dent Assoc 1996;127:1491-1496.
5. Soares IML. Resposta pulpar ao MTA - agregado de trióxido
mineral - comparado ao hidróxido de cálcio em pulpotomias:
estudo histológico em dentes de cães. [Thesis], Brazil: Faculdade
de Odontologia, UFSC; 1996.
6. Pitt Ford TR, Torabinejad M, McKendry DJ, Hong CU,
Kariyawasam SP. Use of mineral trioxide aggregate for repair of
furcal perforations. Oral Surg 1995;79:756-762.
7. Holland R, Souza V, Nery MJ, Otoboni Filho JA, Bernabé PFE,
Dezan Junior E. Reactions of dogs´ teeth to root canal filling with
mineral trioxide aggregate or a glass ionomer sealer. J Endodon
8. Torabinejad M, Hong CU, Lee SJ, Monsef M, Pitt Ford TR.
Investigation of mineral trioxide aggregate for root-end filling in
dogs. J Endodon 1995;21:603-608.
9. Holland R, Souza V, Nery MJ, Otoboni Filho JA, Bernabé PFE,
Dezan Junior E. Reaction of rat connective tissue to implanted
dentin tubes filled with mineral trioxide aggregate or calcium
hydroxide. J Endodon 1999;25:161-166.
10. Torabinejad M, Hong CU, McDonald F, Pitt Ford TR. Physical
and chemical properties of a new root-end filling material. J
Braz Dent J 13(1) 2002
R. Holland et al.
11. Holland R. Histochemical response of amputed pulps to calcium
hydroxide. Rev Bras Pesq Med Biol 1971;4:83-95.
12. Holland R, Pinheiro CE, Mello W, Nery MJ, Souza V. Histochemical analysis of the dogs´ dental pulp after pulp capping
with calcium, barium, and strontium hydroxides. J Endodon
13. Glickman GN, Koch K. 21st-Century endodontics. J Am Dent
14. Holland R, Mello W, Nery MJ, Bernabé PFE, Souza V. Reaction
of human periapical tissue to pulp extirpation and immediate root
canal filling with calcium hydroxide. J Endodon 1977;3:63-67.
15. Holland R, Souza V, Nery MJ, Faraco Júnior IM, Bernabé PFE,
Otoboni Filho JA, Dezan Junior E. Reaction of rat connective
tissue to implanted dentin tube filled with mineral trioxide aggregate, Portland cement or calcium hydroxide. Braz Dent J
16. Faraco Júnior IM. Avaliação histomorfológica da resposta da
polpa de dentes de cães submetida ao capeamento com sistema
adesivo, cimento de hidróxido de cálcio e dois tipos de agregado
de trióxido mineral. [Doctorate thesis]. Araçatuba: Faculdade de
Odontologia, UNESP; 1999.
17. Seux D, Couble ML, Hartmann DJ, Gauthier JP, Magloire H.
Odontoblast-like cytodifferentiation of human dental pulp cells
in vitro in the presence of a calcium hydroxide-containing cement. Arch Oral Biol 1991;36:117-128.
Accepted August 7, 2001
Braz Dent J 13(1) 2002